Sains Malaysiana 44(3)(2015): 429439
Enhancement of Gaseous BTEX Adsorption on RH-MCM-41 by Chlorosilanes(Peningkatan Penjerapan Gas BTEX pada RH-MCM-41 oleh Klorosilana)
T. AREEROB, S. CHIARAKORN* & N. GRISDANURAK
In this research, the surface hydrophobicity of a mesoporous molecular sieve synthesized from rice husk silica, called RH-MCM41 was improved via silylation techniqueto enhance the adsorption efficiency of non-polar volatile organic compound. The effect of chlorosilane leaving on was analyzed with three silanes containing different numbers of chloride leaving group; trimethylchlorosilane (TMCS), dimethyldichlorosilane (DMDCS) and methyltrichlorosilane (MTCS). The unmodified RH-MCM-41 was soaked in 100 mL of 5% v/v of silane reagent at 30C for 24 h. The results showed that the silane loading on the RH-MCM-41 was in the order of increasing number of leaving groups as MTCS > DMDCS > TMCS. The crystallinity results studied by X-ray diffractometry indicated that the silylation did not affect the hexagonal pattern of RH-MCM-41. However, the porosity of the silylated RH-MCM-41 was significantly decreased after silylation, especially by MTCS, due to pore blocking. After silylation, the adsorption performance of gaseous BTEX (benzene, toluene, ethylbenzene and xylene) on the silylated RH-MCM-41 was determined by gas chromatography equipped with flame ionization detector (GC-FID). From the results of humidity effect on adsorbability, the BTEX adsorption capacity of the unsilylated RH-MCM-41 was dropped a half, conversely the BTEX adsorption capacity of all silylated RH-MCM-41 was decreased in range of 20-30% when the relative humidity increased from 25 to 99%. This was indicated that the influence of humidity on the BTEX adsorption was relieved after silylation. In additions, the maximum BTEX adsorption capacity belonged to RH-MCM-41 silylated by TMCS which was recommended for the enhancement of non-polar volatile organic compounds adsorption.
Keywords: Adsorption; BTEX; MCM-41; rice husk silica; silylation
Dalam kajian ini, permukaan kehidrofobian penapis molekul mesoporous disintesis daripada sekam padi silika, dikenali sebagai RH-MCM41 bertambah baik melalui teknik sililasi untuk mempertingkatkan kecekapan penjerapan sebatian organik yang tidak berkutub. Kesan klorosilana yang tertinggal dianalisis dengan tiga silana yang mengandungi jumlah klorida berbeza meninggalkan kumpulan; trimetilklorosilana (TMCS), dimetildiklorisilana (DMDCS) dan metiltriklrosilana (MTCS). RH-MCM-41 yang tidak diubah suai, direndam dalam 100 mL 5% v/v bagi bahana uji silana pada 30C untuk 24 h. Hasil kajian menunjukkan bahawa bebanan silana ke atas RH-MCM-41 adalah dalam aturan penambahan bilangan meninggalkan kumpulan sebagai MTCS > DMDCS > TMCS. Keputusan habluran yang dikaji oleh belauan sinar-x menunjukkan bahawa sililasi tidak menjejaskan corak hexagon RH-MCM-41. Walau bagaimanapun, keliangan sililasi RH-MCM-41 menurun dengan sekata selepas sililasi, terutamanya MTCS, kerana menghalang liang. Selepas sililasi, prestasi penjerapan gas BTEX (benzena, toluena, etilbenzena dan xilena) pada sililasi RH-MCM-41 ditentukan melalui kromatografi gas dilengkapi dengan pengesan pengionan api (GC-FID). Hasil daripada serapan kelembapan menunjukkan kapasiti penjerapan BTEX sililasi RH-MCM-41 jatuh separuh, sebaliknya kapasiti penjerapan BTEX untuk semua sililasi RH-MCM-41 adalah menurun dalam julat 20-30% apabila kelembapan bandingan meningkat daripada 25 kepada 99%. Ini menunjukkan bahawa pengaruh kelembapan pada penjerapan BTEX lebih baik selepas sililasi. Sebagai tambahan, kapasiti maksimum penjerapan BTEX adalah kepunyaan RH-MCM-41 sililasi oleh TMCS yang dicadangkan untuk meningkatkan penjerapan-tidak berkutup organik meruap.
Kata kunci: BTEX; MCM-41; penjerapan; sekam padi silika; sililasi
Nowadays, Mobil composite material number 41 (MCM-41), order mesoporous silica, can be prepared from rice husk silica which is named as RH-MCM-41 (Grisdanurak et al. 2003). The RH-MCM-41 is categorized as a nanoporous material containing silicate framework like honey comb. Its pore diameter is ranged between 20-30 and its surface area is about 700-900 m2g-1 (Chiarakorn et al. 2007). This
material has been introduced to be an alternative adsorbent for the adsorption of various air pollutants, supporting material for catalytic reaction, ion exchange media and filter (Appaturiet al. 2012; Artklaet al. 2009; Beck et al. 1992; Chumeeet al. 2009; Klankawet al. 2012; Tong-On et al. 2009; Wantalaet al. 2010; Yoshitakeet al. 2002; Zhao & Lu 1998). Nevertheless, it was reported that the hydrophilicity of MCM-41 surface caused low adsorbability
when MCM-41 is applied for non-polar volatile organic compounds (VOCs) adsorption under high relative humidity condition (Branton et al. 1999; Idris et al. 2010; Ohashi et al. 1999). This is due to the existence of silanol groups (Si-OH) caused by the hydrolysis of siloxane bond (Si-O-Si) on MCM-41 surface. To resolve this drawback, the surface modification via silylation has been introduced. Generally, the silylation is a well-known technique for surface tailoring on several materials containing silanol groups such as MCM-41, MCM-48, SBA-1 and silica gels (Deschner et al. 2010; Koyano et al. 1997; Lin et al. 2008; Yokoi et al. 2004; Yuan et al. 2006; Zhao & Lu 1998). The common reagents used for the silylation are organosilanes. The silylation reaction takes place by substituting hydroxyl of silanol on MCM-41 surface with hydrophobic alkylsilyl groups (R-Si). It is noticed that the degree of substitution depends on the number of silane leaving groups. We expected that the more alkylsilyl substitution, the more hydrophobicity. However, there are few studies focusing on the silylating techniques and effects of silane functional group on the improvement of hydrophobic surface. For example, Zhao and Lu (1998) modified MCM-41 by trimethylchlorosilane (TMCS) and claimed that the modified MCM-41 was a promising adsorbent for volatile organic compound removal. The study of Patel et al. (2011) also confirmed the enhancement of benzene adsorption in aqueous solution by silylated MCM-41 (Patel et al. 2011). Similar to our previous work, we studied the effect of different alkylsilyl groups on the degree of silylation of RH-MCM-41. Trimethylchlorosilane (TMCS) and phenyldimethylchlorosilane (PDMCS) were used as silane precursors and the ex-situ silylation was applied in this study. The results indicated that a small silane, like TMCS, could improve the hydrophobicity of RH-MCM-41 better than PDMS due to less steric hindrance effect (Chiarakorn et al. 2007). Ketcome et al. (2009) also followed our silylation technique and reported that toluene adsorption efficiency could be significantly improved by RH-MCM-41 modified with TMCS (Ketcome et al. 2009). According to the previous works, the molecular structure of silanes plays the important role in the degree of silylation. We believed that not only the size of alkylsilyl but also the number of leaving groups can affect the silylation reactivity as well as surface properties. The urban area in Thailand has been seriously affected by indoor air pollutants such as benzene, toluene,
ethylbenzene and Xylene (abbreviated as BTEX) which cause diseases including cancer and leukemia to human. Thus, the development of BTEX measurement is urgently required in order to reduce their adverse effects.Thus, this research aimed to study the effect of chlorosilane leaving groups on the silylation efficiency. Three chlorosilanes with different number of chloride leaving groups: Methyltrichlorosilane (MTCS),dimethyldichlorosilane (DMDCS) and trimethylchlorosilane (TMCS) were used as silane reagents. The chemical structures of the silanes were shown in Table 1. The physical and chemical properties of the silylated RH-MCM-41 such as crystallinity, hydrophobicity, porosity and alkylsilyl loading were investigated. The improvement of hydrophobicity was determined by the BTEX adsorption efficiency.
MATERIALS AND METHODS
CHEMICALS AND REAGENTS
All analytical grade reagents used in this study were sodium hydroxide (NaOH 95%, Merck), hydrochloric acid (HCl 37%, Merck), ethanol (C2H5OH 99.8%, Merck), cetyltrimethylammonium bromide (CTAB) ([C16H33N(CH3)3]Br 96%, Fluka), methyltrichlorosilane (MTCS 98%, Fluka), dimethyldichlorosilane (DMDCS 98%, Fluka) and trimethylchlorosilane (TMCS 95%, Fluka).
SYNTHESIS OF RH-MCM-41
In this study bio-silica was used as a silica source for RH-MCM-41 synthesis. The rice husk silica was prepared by the acid extraction adapted from Yalcin and Sevinc (2001) and Boonpoke et al. (2011). Rice husk obtained from rice mill was boiled in 1 MHCl at 80C for 1 h. Then, the pre-treated rice husk was washed with deionized water and then calcined in a muffle furnace at 650C for 4 h. The extracted rice husk silica was mixed with sodium hydroxide and cetyltrimethylammonium bromide (CTAB), which was used as a cationic template, with the molar composition of 1 SiO2: 1.09 NaOH: 0.13 CTAB: 120 H2O. The pH of solution was controlled at 10 and then the solution was stirred for 48 h at room temperature under atmospheric condition (Chiarakorn et al. 2007; Grisdanurak et al. 2003). The white suspended solid was filtered, rinsed with ethanol and distillated water and then calcined at 550C for 5 h. After the synthesis, the physical and chemical
TABLE 1. Chemical structures and molecular weight of silane reagents
Chemical name Trimethylchlorosilane (TMCS)
Molecular weight (g mol-1) 108.64 129.06 149.48
characteristics of the synthesized RH-MCM-41
Click here to load reader